Thermal Expansion of Some Bronzes

Author
shaileshmirasdar 
Category
Documents

view
119 
download
4
Embed Size (px)
Transcript of Thermal Expansion of Some Bronzes
U . S. DEPARTMENT OF C OMMERCE NATIONA L B UREAU OF STANDARDS
RESEARCH PA PER RP1518
Part of Journal of Research of the N ational Bureau of Standards , Vo lume 30, January 1943
THERMAL EXPANSION OF SOME BRONZES By Peter Hidnert
ABST R ACT
The results obtained in the course of independent tests and investigations on the linear thermal expansion of four groups of bronzes designated as tinzinc, leaded, aluminum, and silicon bronzes are given for different temperature ranges. Curves showing the typical expansion and contraction characteristics of these bronzes during heating and cooling are prcsented. Ternary diagrams are given to show the effect of composition on the coefficients of expansion of coppertinzinc and coppertinIead alloys. In general, the coefficients of expansion of these copperbase alloys increase as the addition of tin, zinc, or lead is increased. For the range from 20° to 100° C, the average coefficients of expansion of the various bronzes were found to be between 16.8 X 10 6 and 19.0 X 10 6/° C.
CONTENTS Page
1. Introduction___ _ _ _ __ _ _ _ _ _ __ __ _ _ __ _ __ __ __ _ _ _ _ _ _ _ _ _ _ __ _ _ _ _ _ _ __ _ _ _ _ 75 II . Materials investigated_ _ _ _ _ _ _ _ __ __ _ _ _ __ _ _ _ _ _ _ _ _ _ __ _ _ _ _ _ _ _ _ _ _ _ _ _ _ _ 79
I II. Apparatus____ ____________________________________ _____ ____ _____ 79 IV. Results and discussian_____ ______ ______________________________ __ 79 V. References______________________________________________________ 88
1. INTRODUCTION
During the past 30 years, data on the linear thermal expansion of copperbase alloys designated as tinzinc, leaded, aluminum, and silicon bronzes have been obtained at the National Bureau of Standards. These results are based on independent tests and investigations, the specific purposes of which in general were not related. Therefore, the ranges of temperature within which the bronzes were investigated differed in many cases. These data, together with some previously published results, are summarized in this paper. Ternary diagrams showing the effect of composition on the coefficients of expansion of coppertinzinc and coppertinlead alloys are given.
Available data from previous investigators on the lineal' thermal expansion of various bronzes of known compositions are given in table 1.1 Some of the results in this table, in combination with data of the present paper, were used in the preparation of the ternary diagrams.
1 Data (not liste<l in table 1) from 2 manufacturers have been published by N. L. Mochel, Thermal Expansion of Metals, Symposium OLl Elfect of Temperaturc on the Properties of Metals, Am. Soc. Testing Materials and Am. Soc. Mech . Engrs., p. 683 (1931).
75
TABLE I.Previously published values of coefficients of linear thermal expansion of bronzes by previous observers
Observer Date
Fizeau [11 __ ___________ _ 1 1869
Benoit b [21 ___ ___ __ _____ 1 1889
Le Chatelier [141 ____ _ .1 1889
Dittenberger and 11902 Gehrcke b [3].
Henning «[41 __ ________ _ 1907 Bein b [51 ___ ____ ____ ___ . 1912
Hidnert b [61 ___________ 1 1921
Material
BrOD,ze _______________ _ Bronze ____________ ___ _ ____ do __________ _____ _ _ Phosphor bronze __ __ _ _ ___ _ do ________________ _ ____ do __________ ____ __ _ ____ do ________________ _
{. ~:r:~~r:::::::::::::::: Aluminum bronze 0 _ _ _ Bronze _____________ __ _
. ____ do ________________ _ Bronze k __ ____ do.' ______________ _ Phosphor bronze m ___ _ ____ do ________________ _ Ohain bronze m ______ _ ____ do ________________ _ Bronze ____ do __ __ _____ _______ _ ____ do .m _____________ _ ____ do ___________ __ __ _ _ Aluminum bronze D __ _
___ .do. D ____________  
Cu
% ~3 ~~ ~w ~6 ~6 ~6 ~6 00 ~ m 00 Ul
M 00 ~5 Mm Mm ~. ~. nw nw .~ .~ nu ftU
Hidnert [71 ________ ____ _ 119321 [~,~~d~~p~::::::::::::::1 rs:r Wllkms [81 ______ ______ _ 1933 Silicon bronze Q _______ 94.75
Chemical composition
Sn Zn Pb Ni
Treatment P
Average coefficients of expansion per degree centigrade
0° to I 20° to I 20° to I 20° to I 20° to ~o C 100° C 200° C 3000 C 4000 C Other range
111111 111111% % % % % X 106 X 106 X 106 X 106 X106 1 X 106 9.7 4.0 ______________________________________ >17. 8 _______________________________ _ 9.87 8.60 0.17 ___ ___ _______________ ___ _______ 17.9 ___________________ __ __________ _ 9. 87 8.60 .17 _______________________________ 18.0 ______________________ __ _______ _ 2.2 ____________________ 0.2 H ardened _______ 17.0 _________ ______________________ _ 2.2 ______ ____ ___ _____ __ .2 Annealed _______ 17.0 __ __ _________ _______ ___ ___ _____ _ 4.7 ______ _______ _____ __ . 7 Hardened _______ 17. 4 ________ ___ ____________________ _ 4.7 ______ _______ __ ____ _ .7 Annealed ___ __ __ 17.4 ___________________________________________ _____ __ __ _
10 __ ___ ____ _______ _______ ___ ____ Ao___________ ______ _____ ___ ______ __ ________ ________ 22.0 (00 to 9000 C) 20 _____ _____ ________ _____________ do_____ ______ __ ____ ________ ________ ________ ________ 27.0 (00 to 800° C) 30 ____________________________ __ _ do________ ___ ___ ___ ______ __ ________ ________ ________ 29.5 (00 to 700° C)
_ __ ____ ______ ____ _______ ___ ___ ___ ____ Ao___ ___ _____ ______ __ ____ __ ___ _____ ________ __ ____ __ 23.0 (00 to 9000 C) 6.2 8.7 .7 ___ __ __ ______ __________________ __ ____ __ _____ _ ________ d 18.1 0 18.7 f 19.2
6 26 &5 ~U ~U ~88 ~88 lM ~M
1014 1014
14.95 5.0 0.5
9 0.45
______ , ________ __ __ ___ _ h 18.21 ; IS. 7 17.2 ____ __ ______ __ __ _______ _ 17.5 __________ ____ __ _______ _
__ ___ _ ____ __ _ _______ .37 Cast . _________ __ ___ __ _ ___ __ _ _______ __ ____ _ .37 Co1drolled ____ ______ _ _ ______ _______ _______ .12 Cast ._ . __________ ____ _ ______ _______ ___ ____ . 12 Coldrolled ___________ _ __ ____ ____ __ _ _______ . Il Cast ____ ____ ________ _ _ ______ ____ __ _ _______ . Jl Coldrolled ___ __ _ _____ _ ______ _______ _______ . 00 CasL ___________ __ ___ _ ______ _____ __ __ _____ .00 Coldrolled _____ _ ___ __ _
.40 ___ ____ 'rrace _____ _ Hotrolled ____ ___ _____ _
.40 _________ _ do __ _____ _ Hotrolled and _____ _ drawn.
5.1 1.5
4:~1 1:::::::I : :::::I _~~~~o__:::::::::c::::
17.4 17.S IS.2 17.217.618.0 17.3 17.7 18.1 17.1 17.4 17.S 17.5 U.9 IS.2 17.3 17.8 18.2 17. 7 18. 1 18. 6 17. 6 17. 9 IS. 3 16.5 17.3 IS.2 16.6 17.2 17. 8
18.0 17. 8
r 17.0
18.2 IS. 1
IS.6 18.5
lS.8 18.9
; 19.3
19.3 (200 to 500° C) 19. 3 (20° to 500° C)
~ 0)
"I::> ~
;§ ~ ~ ~ ~ Co ~ ,:, '2
" ;;:,... I::> ........ "'" ;;:,... ~
~ "'" "". I::> ;:;: ,:, "" ~
~ ~ ~ C> ........ V:J
~ ~ ~
Hldnert [91 .. ......... 1 1934
Koiso, Kusu moto, and I 1940 Yata [10].
Bronze ......... . ...... 95.70 1. 95 2.32 .03 CasL . ............... . . ... do.' ............... 82.28 6.70 3.20 7.48 0.15 . 05 ..... do ..... ........... . .... do.'_ . ....... . ..... 88.63 8.58 0.34 2.08 .25 ... .... .... do .. . ...... .. ..... . .... do.' ......... . .. . .. 80. 02 9.58 . 60 9.45 _IS _04 ... . . do ... _ .. ... . ...... . ... . do ......... ..... . . . 86.75 9.97 2.75 0.58 .03 ..... do _ .... . .... _ ... .. . .... do ................. 83.' 80 11.96 4.22 . ...... ..... .. . 02 . .. .. do ..... ......... . . . ... . do .......... ....... 87.75 12.25 . . .. . .... . . .. ........ 02 . .... do ..... ... _._ .. . _ .. Leaded b ronze ,_ ...... 73.00 4. 45 0.25 21. 79 .35 .05 .... _do _ .... .... . _ . .... . .... do ................ . 65.40 7.75 None 26.62 .25 ......... .. do _ ..... ....... . . . . .... do ...... .......... . 69.82 9.72 20.50 .02 ... . _do _ . . ..... _ ....... _ .... do ................. 77.00 11.08 11.90 .02 .. .. . do ....... ...... . .. . . . .. do.'._ ... _ . ... .. ... 75.86 11. 57 _2~ 12.00 .20 .04 . . ... do . ... : ........ ... _ "H B5" bronze u __ __ _ _______________________________________ _
• Coefficieut of expansion at 40° C.
17.2 18. 1 17.5 18. 4 17.8 17.9 17. 7 18. 9 19. 0 18. G 18.6 18. 3 19_1
17.3 t 18.4
17.9 . 18.6
18.3 18.1 18.8 19.0 18.8 18.6 18.7
b Coefficients of expansion compnted from data in original publication. e Aluminum, 10 percent. d From 0° to 250° C.
I Iron, 0.09 percent. m Each coefficient of expansion is t he average of values on 4 sections of a cast rod. n Aluminum 7.34, silicon 0.09 percent.
• From 0° to 375° C . r F rom 0° to 500° C . g Coefficients of expansion compu ted from da ta repor ted by observer. Coefficient of
expansion from 191° to + 16° C, 15.1X10<ljO C_ b F rom 16° to 250° C . ; From 16° to 375° C . ; From 16° to 500° C_ k Manganese, 0.61; iron, 0.22; aluminum, 0.10 percent.
° Coefficient of expansion from 20° to 600° C, 19.8XlO6jO C . • Coefficients of expansion from 20° to 600° C and from 20° to 700° C, 20.0XlOe and
20.GX10<1jO C, respectively. q Silicon, 3.25 percent_ , From 0° to 100° C. 'Antimony, 0.15 percent. t Second hea ting. u Iron, 4; m anganese, 4; zinc, 1 ma.~; chromium, 0.5 max; aluminum, 10.5 percent;
copper, balance.
~ ~
~ ~
~ ~
~ 0'> C ;;3
~
~ ~ ~
bj 'i , C ;;3 (\) ~ ."
.:r .:r
78 Journal of R esearch of the National Bureau of Standards
fz w
~ T ~N zO
~ 1 0.. x W
o
p
p/ / /
"A
/ / /
/ v/ / %/ V
'\~ 0 HEAT IN G ."
./ • COOLI NG •
100 200 300·C TEMPER ATURE
FIGURE l.Linear thermal expansion of two cast tinzinc bronzes.
Sample 376: copper 88, tin 8, zinc 4 percent; sample 895: copper 86.5, tin 11, zinc 2.5, maximum impurities 0.2 percent.
 
Thermal E xpansion oj Some Bronzes 79
II. MATERIALS INVESTIGATED
The samples of bronzes were provided by the American Brass Co., Waterbury, Conn., American Bronze Corporation (now American NonGran Bronze Corporation), Berwyn, Pa., Bridgeport Brass Co., Bridgeport, Conn., E. 1. du Pont de Nemours & Co., Inc., Wilmington, Del., Fredericksen Co. (now Saginaw Bearing Co.), Saginaw, Mich., National Bureau of Standards, Titanium Alloy Mfg. Co., Niagara Falls, N. Y., and W . & L. E. Gurley, Troy, N. Y. The chemical compositions and available information regarding the treatments of the samples are given in table 2. Most of the values for chemical composition were furnished by the manufacturers.
The length of each sample used in the determinations of linear thermal expansion was 300 mm (11.8 in). The cross sections of all samples except those designated as 38 and 39 were circular, with diameters of 8 to 13 mm (0.31 to 0.51 in). The diameter in each case was the same as that of the "as received" rod. Samples 38 and 39, machined to 5 mm (0.20 in.) square section, were cut from bars having a section 16 mm (0.63 in.) square.
III. AP PAR ATUS
The types of precision micrometric thermalexpansion apparatus used for determining the linear thermal expansion of the bronzes are described in previous publications [11, 12, 6, 13).2 In addition to the differences in design, the instruments differed in the ranges of temperature over which they could be operated. However, essentially the same results have been obtained with each of the instruments used for the same ranges of temperature.
IV. RESULTS AND DISCUSSION
Typical expansion and contraction curves for four groups of bronzes are shown in figures 1 to 4. These figures indicate tha t for a relatively narrow range of temperature (fig. 1) the expansion and contraction curves nearly coincide, but in cases involving wider ranges of temperature (figs. 2 to 4) the expansion and contraction curves diverge appreciably. It is of interest to note that the expansion curves in figure 3 indicate that a marked decrease in the rate of expansion occurred in the harddrawn aluminum bronzes at temperatures between 700 0 and 800 0 C. On the other hand, the curves for both the harddrawn and annealed silicon bronzes (fig. 4) showed a marked increase in the rate of expansion between 900 0 and 1,000 0 C.
The average coefficients of expansion of the four groups of bronzes, computed from the expansion and contraction curves (typified by figs. 1 to 4), are given in table 2 for t emperature ranges \vithin which observations were made. The differences in length of most of the bronzes before heating and after passing through the heating and cooling cycle are also shown in this table . In general, the aluminum and silicon bronzes (figs. 3 and 4, and table 2) were investigated over wider ranges of temperature than the tinzinc and leaded bronzes (figs. 1 and 2, and table 2).
2 Figures in brackets indicate tbe literature references at the end of this paper.
497911436
80 Journal of Re8earch of the National Bureau of Standard8
1.0 1071
P
.9
.8
.7
/ fl
I
,;; r' V'I
t .6 z .... //
,P/ '' 0:: .... (L . 5 ~ z 0
.4 ;;; z « (L
x .... .3
/; /
v. I I
/ rf/
/ /
/ / /
/ /
I .2 V I o HEATING / I I
/ • COOLING .1
I I I
I I 0.0
../ • o 100 200 300 400 500·C
TEMPERATURE
FIGURE 2.Linear thermal expansion of leaded bronze (treatment unknown).
Sample 1071: copper 70, tin 9, lead 21, maximum impurities 0.2 percent.
Iz w
~ I z <t
~ I ~ x w
o
Thermal Expansion oj Some Bronzes 81
/ 'l v/ /
/ /,/
// /
 P / I vI /
/
/ /
// /
VI V / , /
/ / , , ,
VI / // , , , ,
~/ / I
" ,
V V V / //
/ / ,
/ I / ,
/
/ v . V VI V
/ "foL.
/ / . V V
/ / / V 0 HEATING
/ / • COOLING
/ /
100 200 300 400 500 600 700 0 800 C
TEMPERATURE FIGURE 3. Linear thermal expansion of two harddrawn aluminum bronzes.
Sample 1416: copper 89.71, tin 0.38, alnminum 9.29, iron 0.44 percent; sample 1417: copper 89.43, tin 0.33, aluminum 9.30, iron 0.58 percent.
l
\
TABLE 2.Coefficients of linear expansion of four groups of bronzes
Chemical composition
Sample
Ou Sn Zn Ph AI SI Mn Fe Other elements
~ ~
1l0L __ I 9~61 {o31 __ 'Yo_L%_L%_L%_L%Jo.,*2 I %
84 ______ _ 90 6.5 308 ______ 88 10 376 ______ 88 8 1068 _____ 87 7 38 ______ _ }S6.7 11.2 39 ______ _
894 ____ __ }86.5 11 895 _____ _
2.0 2 4 5
2.1
1. 5 , _____ , _____ , _____ , ____ _
 i I: : ::: I ::::r::r:~:
2. 5 LII  ILI{~~i~mo~f' impur
Average coefficients of expansion (and contraction a) per degree centigrade
Treatment 20° 20° 20° 20° 200 20° 20° 20° 20° 20° 900° to to to to to to to to to to to 50° 100° 200° 300° 400° 500° 600° 700° 800° 900° 1000° 0 0 0 0 0 0 0 0 0 0 0
_ ._
A. TINZINO BRONZES
Hotrolled and an ~JO;·I ~JO;I ~ _1~~ 1 ~ ~~~ I ~ ~~~~ I ~ ~~~ I ~ ~~~ I ~ ~~J ~ ~~J ~ ~ ~J ~ ~~~ nealed.
Ohang in
lengtb orsam pIe artE heatin
and cooling
r g
% 0.002
Not known _________ 017.4017. 8 ___________ _ _______ _____ ____ ____ _____ ______ _____ ________ _____ _ Oast ________ ___ _______ ___ 17. 8 18.1 18.5 18.8 ______ ______ ___ ___ ______ ______ ___ ___  . 018
_____ do ____________________ 17.S 18.1 IS. 5 _______ ______ ______ ______________ _______ __  . OOi Oast at 2,250° F _____ d17.8 ______ ______ ____ __ ______ ___ ___ ______ ______ ______ ______ __ ____ +. 001
O~~4~~8 (~,~~~~~)d }:g: g :~g :~~: ~ :::::: :::::: :::::: :::::: :::::: :::::: :::::: :::::: :::::::: {O~;I~n g~rna1~~~ } ____ _ 18.1 IS. 3 18.7 ______ ___ ___ ______ ______ ______ ______ ______ .000
2,2500 F.  17.9 18.5 IS.6 _____ _ ______  _____  _____    ___  _____ _____ .001
B. LEADED BRONZES'
00 tv
r ~ ~ ~ Co ~ .::. ~ ;;,..
~ .,... ;;,.. ~
~ .,... ... ~ ~ .::. "" tt1
85 ______ _ 180 r! 1  4I~g 1069 _____ 76
107L __ __ 70 _____ 21  11 11    I Not knowlL 0    1 i loI8. 61 ______ 1 ___ ___ 1 ____ 1 1  1  1  11 1 ~ ::::: ::::: ::::: ::::: FVI;i~~ir'impur }~:t::02:~~ __ ~:: : :: (~:~ : ::: :: : ~~~~: :~~T : ~~~~ : :~fr :::::: :::::: :::::: :::::: :::::: __ ~~~~~ ~
O. ALUMINUM BRONZES'
86 ______ 190
1416 ____ 189. 71 10.38 10.00 1 ____ 19.29
1417 __ ._189.43 I .33 I .00 1 _____ 19.30
_____ , ____ _ , _____ ,10. ''11 ii~~ct~r':::,,;.i;om }  o~~: ~ ~~~~ ~~~8  ~~~~  ~8~; ~;;~~ ~8.;; :::::: :::::: :::::: } ~~.~~ _____ , _____ ,0.44 Nickel 0.18 ________ { ~di. tOt % lll. lU      L '16. 9 *17.7 *18.6 ______ '19.8 '20. 1 20.3 ___________ _
lame er.
I{H ardd rawn frOm} {16 2 164 170 18.0 IS. 6 19.1 g19. 2   } _ 19 ,, .58 I Nickel 0.36_ _______ d~6 tOt % in. in  __ ~ __ *17: 1 *17: 9 '18.6 ____________ *20.0 '20.4 ______ ____ __ .
lame er.
~ UJ §
l
Average coefficients of expansion (and contraction a) per degree Ohang Ohemical composition centigrade in length of sam· Sample Treatment 20° 20° 20° 20° 20° 20° 20° 20° 20° 20° 900° pie afte
to to to to to to to to to to to heating Ou Sn Zn Pb Al Si Mn Fe Other elements 50° 100° 200° 300° 400° 500° 600° 700° 800° 900° 1000° and 0 0 0 0 0 C C C C C C cooling
D. SILICON BRONZES'
% % % % % % % %1 % X10'" XlO6 XlO<I XlO6 X10<l XlO6 X10<l XlO6 XlO6 XlO6 X10'" % 1333 ..... 95.64    0.00       3.04 1. 03 0.09 Harddrawn . ... .. ... ..... 17.217.818.1 17.7 18. 6 19.3 19.820.220.861. h+0.57 1334. .... 95. 64 .00       3. 04 1. 03 .09 Annealed . .... ..... . .... . . 17.4 17.6 18.1 18.2 18. 7 19. 1 19.6 20.1 20.6 64. h+.58 1019 I ....
}9t/"6 151{PhOsPhOrus 0.06, 1020 ..•..    .00      4.0 1.1 1021. .••. . Nickel 0.00. }Not knowL . ...... {tn UJ :::::: :::::: :::::: :::::: :::::: :::::: :::::: :::::: :::::: :88 1394._._. 94. 33             4.40 0.96 .11 ...... Cast { . ... . 17. 4 17. 5 18.0 18.2 18.9 19.8 20.6 21. 1 21.7 . ..... } _ 13
. . .. ..... . ..... . . .... *16. 3 *17.3 *17.9 .. .. .. 'lB. B . •• •.. ••.•. . *21. 0 *23.1 ...... .
a Coefficients of contraction on cooling are indicated by asterisks. b Determined from the expansion curve on heating and the con traction curve on
cooling. The plus sign indicates an increase in length and the minus sign a decrease in length.
o Determined by A. W. Gray, formerly of the National Bureau of Standards. d From 20° to 40° C. Coefficients of expansion per degree centigrade from 20° to
0°,0° to +20°, and 0° to +40° C were found to be 17.0XlO6, 17.0XlO<I, and 17.4XlO<I, respectively.
• From 20° to 150° C, determined by A. ,v. Gray.
(From 20° to 40° C. Coefficients of expansion per degree centigrade from _20° to 0°, 0° to +20°, and 0° to +40° C were found to be 17.1X1Q<!, IB.1XlO6, and 18.2XIQ<!, respectively.
g From 20° to 650° C. h Change in length determined from length measurements on a duplicate sample
before and after heating it to 1,000° C and cooling to 20° C. i Chemical compOSition determined by G. F. Commisa, of the National Bureau of
Standards.
~ '" ~ ~ .... ~ ~
§ "" <" . <::> ;::!
~
~ ~ '" ~ ;::! l\l
'" ""
00 C/.:I
84 J ournal of R esearch of the National Bureau of Standards
IZ W ()
~ T z v
o z
I o U; L Z Cf: x w
o
~ , : : .
I
! /? , ,
, , ,/ I , ,
, I
,/ "
/ ,
;/
/ ~,~
/ // V? / V/ ~/('
~"V / V/// ~
~x; ~~ t" ~'?' ~// I / ~~;; ./
/ / /. V/
I / ~4;i //
// / V' I
~ // ,"0
./ /' 'i / 0/ / ~
/ 'i I / ~ ,"i
/ :/ 0 HEAT I NG
• COOLING
/ 100 200 300 4 00 500 600 700 800 900 1000 C
TEMPERATURE FIGURE 4.Linear thermal expansion of three silicon bronzes.
Sample 1394: copper 94.33, silicon 4.40, manganese 0.96, iron 0.11 percent; samples 1333 and 1334: copper 95.64, silicon 3.04, manganese 1.03, iron 0.09 percent . •
Thermal Expansion oj Some Bronzes 85
The ternary diagrams in figure 5 show the influence of additions of tin and zinc on the coefficients of expansion of coppertin and coppertinzinc alloys for three ranges of temperature. The effect of different contents of tin and lead in leaded bronzes is shown in a similar manner
PERCENT TIN
2 4 G 8 10 14 PERCENT TIN
FIGURE 5.Portions of trianJular diagTams indicating the effects of composition on the coefficints of expansion (in millionths per degree centigrade) of coppertin and coppertinzinc alloys.
C=Cast. CA=Cast and annealed. CR= Coldrolled.
II = Hotrolled. IIA = HotrolIed and annealed. IID=Hotrolled and dl'Rw.6.
in figures 6 and 7. These figures are based on the data in table 2 and previously published results of the author [6, 7, 9]. These diagrams show, in general, that the coefficients of expansion of the bronzes increase as the content of these addition elements is increased.
86 Journal 01 R esearch 01 the National Bureau 01 Standards
4 8 12 16 20 24 28 30 PER CENT TIN
FIGURE 6.Portion of triangular diagram indicating the effects of composition on the coefficients of expansion (in millionths per degree centigrade) of coppertin and coppertinlead allays between 20° and 100° C.
C=Cast. CR=ColdrolIed_
H=HotrolIed.
HA = Hotrolled and annealed . HD=Hotrolled and drawn.
X=Treatment unknown.
Thermal Expansion of Some Bronzes
4 8 12 16 20 24 28 30 PERCENT TI N
87
FIGURE 7.Portion of triangular diagram indicating th., effects of composition on the coefficients of expansion (in millionths per degree centigrade) of coppertin and coppertinlead alloys between 200 and 2000 c.
C=Cast. HD =Hotrolled and drawn. CR= Cold·rolled. X ='l"'reatment unknown.
H=Hotrolled.
88 Journal of Re8earoh of the National Bureau of Standard8
The limiting coefficients of expansion of different bronzes for three temperature ranges are given in table 3.
In cases where comparison was possible, the data presented in this paper were found to be in good agreement with the results of other investigators.
TABLE 3.Ranges of coefficients of linear expansion a of various bronzes
Alloys
Coppertin (0 to 15.0% tin) _________ _________ ____________ _ Coppertinzinc (8 to 12% tin, 2 to 4% zinc) ______ ______ _ _ Coppertinlead (2.0 to 11.6% tin, 2.1 to 26.6% lead) ____ _ _ Coppertinzinclead (5.0 to 6.7% tin, 2 to 5.1% zinc, 1.5 to
7.5% lead) . . Copperaluminum (7.3 to 10% aluminum) ______________ _ Coppersilicon b (3.0 to 4.4% silicon) ____________________ _
Average coefficients of expansion per degree centigrade
20° to 100° C. 20° to 2000 C. 20° to 300° C.
X 1016.B to IB.O 17.B to IB.l 17.2 to 19.0 17.8Jo l B. l
16.2 to 17.1 17.20 to 17.4
XIG' 17.2 to IB.2 lB.l to lB.5 17.3 to 19.9 18.1 to lB.4
16.3 to 17.3 17.5' to 17.B
XlO17.6 to IB.6 lB.5 to lB.7
16.8 to lB.2 lB.Oo to lB. 1
• Data from previous publications by the author [6, 7, 9] were also used in the preparation of this tahle_ b Con tain 1% manganese. o Coefficients of contraction of a cast 4.4% silicon hronze were found to be 16.3XI06, 17.3Xl()o, and
17.9XI0 for the ranges 1000 to 20° C, 200° to 20° C, and 300° to 20° C, respectively.
V. REFERENCES [1] H_ Fizeau, Tableau des dilatations par la chaleur de divers corps simples metal
liques, ou non metalliques. et de quelques composes hydrogenes du carbone, Cornpt. rend. 68, 1125 (1869)_
[2] R. Benoit, Comparaisons de regles metriques et meSU1'es de dilatations, J_ phys. 8, 451 (1889).
[3] Dittenberger a nd Gehrcke, Die Thatigkeit der PhysikalischTechnischen Reichsanstalt irn Jahre 1901, p . 112. (See also W. Dittenberger, ueber die Ausdehnung von Eisen, Kupfer, Aluminium, Messing und Bronze in hoher Temperatur, .Z. Ver. deut. lng. 46, 1532 (1902).)
[4] F. Henning, Uber die Ausdehnung fester I(orper bei tiefer Temperatur, Ann. Physik 327, 631 (1907).
[5] W. Bein, Ausdehnungsbestimmungen am AbbeFizeauschen Dilatometer, Verhandl. deut. physik. Ges. 14, 1097 (1912) .
[6] P. Hidnert, Thermal expansion of copper and some of its important industrial alloys, BS Sci. Pap. 17, 91 (1922) S410.
[7] P. Hidnert, Thermal expansion of copper alloys, Phys. Rev. 39, 551 (1932). [8] R. A. \\filkins, Herculoy, A coppersilicontinzinc alloy, Metals & Alloys 4,
123 (1933). [9] P. Hidnert, Thermal expansion of bearing bronzes, BS J . Research 12, 391
(1934) RP665. [10] G. Koiso, K. Kusumoto, and M. Yata, Some corrosionresistant wrought
aluminum bronzes of high strength, T etsutoHagane 26, 537 (1940). Abstracted in Chern. Abstracts 35, 422 (1940).
[11] A. W. Gray, A new type of apparatus for measuring linear expansion, Phys. Rev. 34, 139 (1912).
[12] A. W. Gray, New methods for displacement measurements and temperature uniformity applied to the determination of linear expansivity, J. Wash. Acad. Sci. 2, 248 (1912).
[13] W. Souder and P. Hidnert, ~Measurements on the thermal expansion of fused silica, BS Sci. Pap. 21, 1 (192627) S524.
[14] H. Le Chatelier, Sur la dilatation des metaux aux temperatures elevees, Cornpt. rend. 108, 1096 (1889).
WASHINGTON, October 22, 1942.
o
KATIONAL BUREAU OF STANDARDS, WASHINGTON, D. C.
Send me the Mathematical Tables marked X below. I enclose remittance 1 to cover the cost.
Mark X Title of publication
MTl. Tahle of the first ten powers of the integers from 1 to 1000 _____________ _ MT2. Tables of the exponential function ex ________________________________ _ MT3. Tables of circular and hyperbolic sines and cosines for radian arguments __ _ MT4. Tables of sines and cosines for radian arguments ______________________ _ MT5. Tables of sine, cosine, and exponential integrals, volume L _____________ _ MT6. Tahles of sine, cosine, and exponential in tegrals, volume 1L ____________ _ MT7. Table of natural logarithms, volume L ________ _______________________ _ MTS. Tables of probability functions, volume L ____ ______________ __________ : MT9: Table of natural logarithms, volume 1L ______________________________ _ MTIO. TalJle of natural logarithms, volume IIL ___ ______ ___ ___________ _____ _ M T11 . Tables of moments of inertia and section modulL ____________________ _ MT12. Table of natural logarithms, volume IV _____________________________ _ MT13. Table of sine and cosiI)e integrals __ _________ _____________________ ___ _ MT14. Tables of probability functions, volume 1L __________________________ _ MT15. Th e hypergeometric and Legendre functions with applications to integral
equations of potential theory ________________________________ __ __ _
Price
United States and its possessions, and countries ex· tending franking privilege
$0. 50 2. (10 2. 00 2. 00 2. 00 2. 00 2. 00 2. 00 2. 00 2. 00 2. 00 2. 00 2. 00 2. 00
2. 00
Amount enclosed Other countries
$0. 65 ____________ 2. 50   2. 50   2. 50 2. 50  2. 50  2. 50 2. 50 2. 50 2. 50  2. 50  2. 50   2. 50  2. 50  2. 50  
Total remittance _____________________________ ___ ____ _______________ , ______________ , ___________ _
1 Remittance should be in form 01 postoffice money order, or check, and made payable to the order of the "National Bureau of Standards" in United States currency.
Send to _____ ________ ___ _____ _______________________ _________________________________________________ __ ___ __ : ____________ _
Number and Street _____ ______________________ ____________________________________________________________________________ _
City and State ______ ~ __________________________________________________________________________________________________ __ _
(Cut bere) /
MATHEMATICAL TABLES
Attention is invited to a series of publications which is being prepared by the Project for the Computation of Mathematical 'Tables conducted by the Federal Works Agency, Work Projects Administration for the City of New York under the sponsorship of the National Bureau of Standards. To date, 14 tables have been made available through the National Bureau of Standards. These are listed below:
There is also included in this list a publication on the hypergeometric and Legendre functions (MT15), prepared by the Bureau.
MTl. TABLE OF THE FIRST TEN POWERS OF THE INTEGERS FROM 1 TO 1000:
(1938) VIII + 80 pages; heavy paper cover. 50 cents.
MT2. TABLES OF THE EXPONENTIAL FUNCTION e%:
The ranges and intervals of the argument and the number of decimal places in the entries are given below :
Range of x  2.5000 to 1.0000
1.0000 to 2.5000 2.500 to 5.000 5.00 to 10.00
Interval of x 0.0001
.0001
.001
.01
(1939) XV + 535 pages; bound in buckram, $2.00.
Decimals given 18 15 15 12
MT3. TABLES OF CIRCULAR AND HYPERBOLIC SINES AND COSINES FOR RADIAN ARGUMENTS:
Contains 9 decimal place values of sin x, cos x, sinh x and cosh x for x (in radians) ranging from o to 2 at intervals of 0.0001.
(1939) XVII+405 pages; bound in buckram, $2.00.
MT4. TABLES OF SINES AND COSINES FOR RADIAN ARGUMENTS:
Contains 8 decimal place values of sines and cosines for radian arguments ranging from 0 to 25 at intervals of 0.001.
(1940) XXIX+275 pages; bound in buckram, $2.00.
lI1T5. TABLES OF SINE, COSINE, AND EXPONENTIAL INTEGRALS, VOLUME I:
Values of these functions to 9 places of decimals from 0 to 2 at intervals of 0.0001. (1940) XXVI+444 pages; bound in buckram, $2.00.
MT6. TABLES OF SlNE, COSINE, AND EXPONENTIAL INTEGRALS, VOLUME II: Values of these functions to 9, 10, or 11 significant figures from 0 to 10 at intervals of 0.001
with auxiliary tables.
(1940) XXXVIH 225 pages; bound in buckram, $2.00.
MT7. TABLE OF NATURAL LOGARITHMS, VOLUME I:
Logarithms of the integers from 1 to 50,000 to 16 places of decimals. (1941) XVIII + 501 pages; bound in buckram, $2.00.
MT8. TABLES OF PROBABILITY FUNCTIONS, VOLUME I:
Values of these functions to 15 places of decimals from 0 to 1 at intervals of 00001 and from 1 to 5.6 at intervals of 0.00l.
(1941) XXVIII + 302 pages; bound in buckram, $2.00.
[Continued on p. 4 of coved
[Continued from p. 3 of cover J
MT9. TABLE OF NATURAL LOGARITHMS, VOLUME II:
Logarithms of the integers from 50,000 to 100,000 to 16 places of decimals. (1941) XVIII + 501 pages; bound in buckram, $2.00.
MTlO. TABLE OF NATURAL LOGARITHMS, VOLUM!! III:
Logarithms of the decimal numbers from 0.0001 to 5.0000, to 16 places of decimals. (1941) XVIII+501 pages; bound in buckram, $2.00.
MT 11. TABLES OF THE MOM!!NTS OF IN!!RTIA AND SECTION MODULI OF ORDINARY ANGLES CHANNELS, AND BULB ANGLES WITH C!!RTAlN PLAT!! CoMBINATIONS:
(1941) XIII+197 pages; bound in green cloth. $2.00.
MT12. TABLE OF NATURAL LOGARITHMS, VOLUME IV:
Logarithms of the decimal numbers from 5.0000 to 10.0000, to 16 places of decimals. (1941) XXII+506 pages; bound in buckram, $2.00.
MT13. TABLE OF 5lN!! AND CoSlNB INT!!GRALS FOR ARGUM!!NTS FROM 10 TO 100:
(1942) XXXII + 185 pages; bound in buckram, $2.00.
MT14. TABLES OP PROBABILITY FUNCTIONS, VOLUME II:
Values of these functions to 15 places of decimals from 0 to 1 at intervals of 0.0001 and from 1 to 7.8 at intervals of 0.001.
(1942) XXI+344 pages; bound in buckram, $2.00.
MT15. The hypergeometric and Legendre functions with applications to integral equations of potential theory. By Chester Snow, National Bureau of Standards. Reproduced from original handwritten manuscript.
(1942) VII + 319 pages; bound in heavy paper cover. $2.00.
Payment is required in advance. Make remittance payable to the "National Bureau of Standards", and send with order, using the blank form facing page 3 of the cover.
The prices are for delivery in the United States and its possessions and in countries extending the franking privilege. To other countries the price of MTI is 65 cents; that of MT2 to'MT15, inclusive, is $2.50 each; remittance to be made payable in United States currency.
Copies of these publications have been sent to various Government depositories throughout the country, such as public libraries in large cities, and colleges and universities, where they may be consulted.
A mailing list is maintained for those who desire to receive announcements regarding new tables as they become available. A list of the tables it is planned to publish will be sent on request.